large area ir microlens arrays of chalcogenide glass ... papers/prabhat...large area ir microlens...
Embed Size (px)
Large Area IR Microlens Arrays of Chalcogenide Glass Photoresistsby Grayscale Maskless LithographyYogeenth Kumaresan, Amritha Rammohan, Prabhat K. Dwivedi, and Ashutosh Sharma*
Department of Chemical Engineering, Indian Institute of Technology Kanpur, Kanpur 208016, India
ABSTRACT: The ability to use chalcogenide glass thin filmsas photoresists for one-step maskless grayscale lithographicpatterning is demonstrated. It is shown that the chalcogenidephotoresists can be used to fabricate grayscale patterns withsmooth and continuous profiles such as arrays of cylindricaland spherical microlenses, which are useful as opticalstructures for IR applications. The etching and exposureparameters are optimized to obtain smooth reproducible lensarrays of 150 μm periodicity and up to ∼170 nm height onlarge areas (∼1 cm2). The roughness is found to increase as afunction of the exposure dose and is attributed to the selectivedissolution of the As−Se, As−As, and Se−Se bonds present inthe nanodistributed phases and the presence of the oxide phase. Thus, a minimum exposure dose produces optimally patternedlens arrays. The focal length calculated for the smooth microlens array is ∼9.3 mm, indicating the suitability of the lens arrays forfocusing applications in the IR region.
KEYWORDS: chalcogenide glass, thin film, grayscale lithography, microlens arrays, photopatterning, maskless lithography
Chalcogenide glasses have become promising materials for avariety of infrared optics (IR) applications based on thephotoinduced effects that these materials exhibit.1−5 One of themost interesting of these properties is the change in thechemical resistance to various solvents on exposure to light ofappropriate wavelength and intensity.6,7 This property allowsthe use of these materials as inorganic photoresists inphotolithography. Chalcogenide photoresists have severaladvantages over polymer-based organic photoresists becauseof their smaller fundamental structural units and strongcovalent bonds that makes lithographic patterning of smalland robust 3D features possible.8,9 Deposition of chalcogenideglasses over large homogeneous areas with a low concentrationof chemical inhomogeneities is also achievable by techniquessuch as thermal evaporation and sputtering.10 It is alsoimportant to note that the pre-baking and post-baking stepsof polymer photoresist-based lithography are also eliminated.Photoresist properties together with high transmission in the IRregion are advantageous for creating microlens arrays andoptical gratings for application in medical tomography, opticalcommunication, CCD cameras, and microimaging sys-tems.10−12 These periodic lens arrays also have a reduceddepth of focus as compared to a single lens and can thus reducedevice size when employed in micro-optical devices.13
However, the widespread use of these structures requires areliable and high-resolution fabrication technique to reprodu-cibly construct high quality defect-free 3D structures. The maintechniques for fabricating microlens arrays are based onchalcogenide photoresists such as As2S3, As2Se3, Ge10Se50As40,
and As10S60Ge30.1,14−16 They have been used as negative or
positive type inorganic photoresists based on the specificsolvent used as the developer.8 However, for fabrication of trulycurved and optically smooth structures such as lenses, theconventional planar or 2D techniques of lithography are notsuitable. Thus, fabrication of microlens arrays in these materialsrequires novel adaptations of lithographic techniques.Eisenberg and co-workers have developed various litho-
graphic techniques for the fabrication of 3D structures inchalcogenide photoresists such as proximity lithography,grayscale mask lithography, and thermal reflow.15−18 In theproximity method, one major limitation inherent to thetechnique is the low fill factor of the microlens due to thelateral spreading of the light. In the thermal reflow method,fabricated microlenses are required to be transferred on asuitable substrate by using anisotropic etching. However, manyparameters have to be optimized in anisotropic etching to getthe desired pattern. Halftone or continuous tone grayscalemask lithography used by Eisenberg et al.19 involves the use of aphysical grayscale mask having a light transmission gradient,which is usually fabricated by expensive techniques. This maskis then used in the contact mode to directly fabricate a designedshape in chalcogenide photoresists. Other techniques used tocreate optical elements using chalcogenides include softlithography,20 holographic techniques,21 and interference
Received: April 17, 2013Accepted: July 5, 2013
© XXXX American Chemical Society A dx.doi.org/10.1021/am401368e | ACS Appl. Mater. Interfaces XXXX, XXX, XXX−XXX
photolithography,22,23 etc., which involve multiple or compli-cated steps or expensive equipments.Recently, Kovalskiy et al.14 have used high-energy beam-
sensitive (HEBS) blank glass masks created by e-beamlithography for fabrication of the lens arrays. They used thesemasks along with a mask aligner to expose thermally depositedAs−S thin films followed by wet and dry negative etchingprocesses. It was found that surface roughness of the dry etchedfabricated structures is undesirably high. The fabrication of theHEBS mask and exposure by e-beam are time-consumingprocesses, especially for thicker films. As compared to e-beamor other serial writing techniques, a parallel technique wherethe entire substrate is exposed at once is more advantageous.We have previously demonstrated a grayscale maskless
lithographic technique for the fabrication of 3D structures ina SU-8 photoresist in a single lithographic step.24 Wedemonstrate here the application of grayscale masklesslithography to a chalcogenide photoresist for the facilefabrication of 3D microlens arrays in a single lithographicstep. Here, the light intensity incident on the photoresist isscaled by a grayscale value that ranges from 0 (black) to 255(white) on a digital image file. This grayscale value is translatedinto variation in light intensity incident on a photoresistthrough a digital micromirror device (DMD) consisting of anarray of micromirrors that can be rapidly reconfigured bysoftware and can pattern over an area of ∼1 cm2.24 Anintermediate exposure intensity in proportion to the grayscalevalue is obtained by controlling the ratio of the time amicromirror reflects UV light onto the photoresist to the totaltime of exposure. The x−y patterning is achieved by creatingcomputer generated images with regions varying in grayscalevalue. We thus demonstrate patterning of chalcogenidephotoresists thin films in a single lithographic step by usingthe grayscale capabilities of the maskless exposure system.Further, we explore the mechanism responsible for the creationof roughness and optimize the lithographic parameters such asthe developer, developing time, and exposure dose to obtainrelatively smooth and truly curved reproducible periodicstructures such as convex and concave microlens arrays in asingle lithographic step.
2. EXPERIMENTAL PROCEDUREAmorphous thin films of As40Se60 with various thicknesses (∼0.2−2.0μm) were prepared from commercially available bulk chalcogenideglasses obtained from VITRON GmbH, Germany. Films wereprepared by thermal evaporation (HHV, India, model 12A4D-T)onto rotating substrates at room temperature. Precleaned microscopicglass slides (RivieraTM, India) and silicon wafers (Wafer World, Inc.,U.S.A.) were used as substrates. The glass slides and Si wafers were cutinto approximately 1 in. × 1 in. squares prior to deposition. Thedeposition rate of the films in a vacuum of 2 × 10−6 Torr wascontrolled to ∼10 nm/s. The substrate holder was rotated at frequency∼3 Hz during the deposition to produce uniform films of 2 μmthickness. The films were annealed for 2 h at 150 °C for stabilizing thefilms prior to conducting exposure experiments.The field emission scanning electron microscope (Carl Zeiss, Supra
40 VP) and attached energy dispersive X-ray analyzer (Oxford, U.K.;spatial resolution 0.5 μm radius) were used to confirm thehomogeneity of surface topography and the chemical compositionon different spots of the films. The data over six points were averagedfor surface composition across the film. Confocal Raman spectroscopy(Witec) was used to observe the chemical homogeneity across thedepth of the films. The amorphous nature of the films was checked bymeans of the X-ray diffraction measurements (PAN alytical, TheNetherlands). All the samples were stored in complete darkness and in
a clean and moisture-free, glovebox (VAC, U.S.A.) environment toprevent them from possible oxidation and/or exposure. The annealedchalcogenide samples were cleaned with nitrogen blowing and wereheated to 50 °C to remove adsorbed moisture prior to exposure. TheUV irradiation of the films was done in clean room environment(Class 100) by mercury lamp (power density ∼15 mW/cm2) attachedto a maskless lithography system (SF-100 from Intelligent Micropatterning LLC, St. Petersburg, FL). The grayscale software mask wasdesigned in Microsoft bitmap software. The power density of themercury lamp was measured with a UV power meter (model 306,OAI, U.S.A.). The exposure setup was calibrated such that each pixelin the electronic file corresponded to an area of 15 μm2 on thephotoresist substrate. The exposure light intensity is given by the RGB(red, green, and blue) code of the color used to fill a specific pattern. Areproducible grayscale was implemented by setting the red, green, andblue all to the same value between 0 and 255 (0 for black and 255 forwhite). The grayscale software mask was prepared by varying the valuebetween 0 and 255 in order to obtain the curve shaped structure.Exposure time used for the samples was varied from 900 to 3600 swith lamp power density measured at 15 mW/cm2 for blank whitelight. The dose delivered to each 15 μm2 area of the sample is afunction of the grayscale RGB value of the corresponding pixel andexposure time. Lens arrays of more than 4000 lenses over an area of 1cm2 could be exposed on the As2Se3 thin film.
Exposed films were developed in different amine-based developersethanolamine, butylamine, and propylamine (Fisher Scientific, India)in a glass beaker for up to 3 min with constant agitation. Afterdevelopment, the samples were rinsed in IPA (isopropyl alcohol,Fisher Scientific, India) and dried using a nitrogen gun. For dissolutionkinetics, the difference in height between the exposed and unexposedregion was plotted as etch depth. All samples were analyzed using bothan optical microscope (Leica, DM 2500 M) and field emissionscanning electron microscope (FESEM). Surface profiling of thefabricated lens structure was carried out using an optical profilingsystem (NanoMap-D, Aep Technlogy, U.S.A.) and the thicknesses ofthe developed films were characterized using an atomic forcemicroscope (AFM) from Agilent PICOSPM II.
3. RESULTS AND DISCUSSION
3.1. Characterization of As-Deposited and AnnealedFilms. The chemical composition and distribution of phases inthe as-deposited and annealed films were characterized beforesubjecting to lithographic treatment. This can serve as thereference to understand the effect of grayscale exposure on thechemical properties of the As2Se3 films. The chemicalcomposition of the as-deposited films was analyzed by EDAX(energy dispersive X-ray analysis) measurements at differentpoints on the surface of the film. The data averaged across sixpoints showed an over stoichiometric amount of As (41.4 at %in film as compared to bulk 40 at %) and substoichiometricamount of Se (films: Se 58.2 at %, bulk 60 at %) possibly due tothe higher volatility of selenium as compared to the arsenic.25 Anegligible amount of oxygen was observed on the surface byEDAX. The chemical nature of the films was previouslyanalyzed by us using Raman spectra measurements.26 The As−As, Se−Se, and As−Se bond peaks and peaks arising from Serings, etc. were confirmed. In addition, we have also found thatthe peaks observed using confocal Raman spectroscopy atdifferent depths of a single film appear to be constant indicatingchemical homogeneity across the depth of the 2 μm thick film.Furthermore, the amorphous nature of the annealed films wasalso confirmed by the absence of sharp peaks in the XRD graph(results not shown).
3.2. Grayscale Lithographic Scheme. Chalcogenide thinfilms undergo photostructural changes when exposed to UVlight. Exposed areas of the films are selectively protected from
ACS Applied Materials & Interfaces Research Article
dx.doi.org/10.1021/am401368e | ACS Appl. Mater. Interfaces XXXX, XXX, XXX−XXXB
the etchant in proportion to the irradiation dose as is the casewith all negative photoresists. Grayscale lithography is based onthe fact that not only the exposure time but the light intensityalso affects the selective protection. Figure 1 shows a scheme of
the grayscale lithography for the patterning of convex sphericallens arrays in chalcogenide glasses. The first step is thedesigning of a suitable digital mask for lenses. Considering theprocess for a negative photoresist, thicker regions are created byhaving corresponding regions in the digital mask that transmitmore light, and thinner regions are created by having regionsthat transmit less light in the mask. This graded exposure causesphotoinduced changes that affect the structure and ordering ofthe chalcogenide film.27 The desired micropattern is obtainedby developing with a suitable selective solvent.Another effect of the exposure of chalcogenides to light is the
photo expansion effect, i.e., the increase in dimensions onexposure to light. Various researchers have encountered thisphenomenon. Tanaka et al.28 found a photo expansion of an∼5% increase in the As2S3 flake of thickness 50 μm byirradiating with a 632.82 nm He−Ne laser and focusing a 2.0eV light of 103 W/cm2 intensity. Bishop and co-workers29 havealso reported a photo expansion as high as 10% of the irradiatedvolume using 514 nm light (photo energy = 2.41 eV) from anArgon iron laser. Photo expansion in these disks of As2S3depends on the source and intensity used for irradiation. In ourcase, a lamp (i line 365 nm, g line 436 nm) having maximum 15mW/cm2 power density was used for exposure with a grayscalemask to minimize the photoexpansion effect. To verify this, weexposed one part of the annealed film using a UV light sourcefor the maximum time (3600 s) and covered other part withTeflon to avoid exposure. After exposure, we measured theheight difference between two regions (exposed andunexposed) using an optical profilometer. The height differencebetween two regions was found to be of negligible magnitude.Thus, under the exposure conditions employed in all theexperiments, a negligible photo expansion is to be expected.3.3. Grayscale Lithography: Effects of Developing
Solution and Developing Time. A suitable developer can bechosen based on many criteria such as safety of use, defect-freeetching, selectivity, etc. However, for grayscale lithography, asensitive developer is required to proportionally etch regionsexposed with closely varying grayscale intensity values. Agreater range of profile heights can thus be patterned. Thesensitivity of a developer is characterized by the ratio of therates of etching of exposed and unexposed areas. Furthermore,if a developer with fast dissolution kinetics is used, then theetch profile is not determined by the developing parameters.
Instead, it is predominantly a function of the exposure intensityor the grayscale value at a region alone.To find an optimal developer for grayscale lithography, we
considered three primary amines: ethanolamine, propylamine,and butylamine. Manevich et al.18 and Bryce et al.10 havealready reported amines as a good negative etchants for As2Se3.The mechanism of selective etching of exposed and unexposedregions is due to the differential etching of homopolar andheteropolar bonds in the As2Se3 films. Regions exposed to UVhave been found to have a higher concentration of heteropolarbonds of the As−Se type that are more resistant to etching byamine developers. Hence, amine developers with As2Se3 filmscreate the negative photoresist combination.30,31 To understandthe dissolution kinetics of the three developers, we exposedannealed As2Se3 films to white exposure for 1800 s anddeveloped each of the samples in a different developer solution.The etch depth was measured by optical profilometry at regularintervals as shown in Figure 2. From the graph, it is apparent
that after 3 min, the saturation etch depth is reached for thecase of ethanol amine, while the etch depth in the case of butyland propyl amine shows a linearly increasing trend. Thus, in thecase of ethanol amine, we can expect the saturation depth ateach grayscale value to be reached within 3 min and not vary asa function of the developing time. On the other hand, in thecase of propyl and butyl amine, it takes a longer time forsaturation depth to be reached, and hence, the etch profiledepends on the developing time as well as grayscale intensity ofexposure.This difference in dissolution kinetics across the different
primary amines is due to the difference in polarity of thesolvent.30−32 Butylamine being the strongest base has thelowest polarity, while ethanolamine has the highest polarityamong the three primary amines. Thus, the dissolution reactioninvolving ethanolamine is fastest among the three solvents. Infurther experiments, ethanol amine was used as the developer.Next, to understand the sensitivity of the developer to the
exposed and unexposed regions, we exposed an annealedAs2Se3 film to blank (white) exposure for 900 s. The exposedfilm and a control unexposed film were then developed inethanolamine. Their etch depths were measured using opticalprofilometry at regular intervals as shown in Figure 3. Asexpected, the etch depth of unexposed film decreases fasterthan that of the exposed film. The complete dissolution of anunexposed region of an ∼800 nm height takes around 3 min.Also, the maximum difference in the height between theexposed and unexposed etch depths is also at ∼3 min. Hence, adeveloping time of 3 min is found to be the optimumdeveloping time for the As2Se3 films.
Figure 1. Schematic of grayscale lithography for As2Se3 chalcogenidephotoresist.
Figure 2. Etch depth variation with increasing developing time inethanolamine, propylamine, and butylamine.
ACS Applied Materials & Interfaces Research Article
dx.doi.org/10.1021/am401368e | ACS Appl. Mater. Interfaces XXXX, XXX, XXX−XXXC
3.4. Grayscale Lithography: Effect of Exposure Dose.After the developer and developing time were fixed to theirnear optimal values, the effect of exposure dose, i.e., exposureintensity or grayscale value and exposure time, was analyzed. Inthe first set of experiments, four different As2Se3 thin films withthickness of ∼2 μm were exposed for 900, 1800, 2700, and3600 s with blank white exposure. The films were thendeveloped in ethanolamine for 3 min according to ourpreviously optimized developing parameters. The heights ofthe films were measured using AFM and are plotted in Figure 4
as a function of exposure time. We note from the result that theheight of the film after developing is roughly proportional tothe exposure time. An exposure time of 3600 s was sufficient toobtain 700 nm high films. While a higher exposure time wouldresult in taller structures, we expect that defects would increase.Exposure systems usually also have limitations of maximumcontinuous exposure for maintaining stable light intensities.Hence, we have used a maximum exposure time of 3600 s.Using the limit of exposure time of 3600 s, as-deposited
As2Se3 films were exposed using a grayscale pattern. A grayscalesoftware mask was designed by areas of lighter grays (highergrayscale or RGB value) where a taller structure was desiredand darker grays (lower grayscale value) where shorterstructures were desired. Concave cylindrical lens arrays werefabricated by using alternating black and white strips withgradually varying grayscale values in between the two in thesoftware mask as shown in the inset of Figure 5a. Figure 5ashows the Brightfield microscope image of an array of concavecylindrical microlenses exposed for 3600 s. Figure 5b shows theoptical profilometer image of the cylindrical microlens array.The profile clearly proves the grayscale patterning of
chalcogenides by showing heights proportional to regions of
grayscale. Regions with lighter grays are higher than regions oflower grayscale values with maximum values of 700 nm at thewhite regions. The profile also shows the regular and uniformperiodic structures, indicating that the heights are reproduciblewith respect to the corresponding grayscale value. This meansthat once the lithographic parameters are fixed the etch depthor pattern height is a function only of the grayscale value, andthis information can be extrapolated to any desirable structure.The profile also shows a relatively smooth curved structurewithout any digitization of height. This is due to the softcontrast characteristics in grayscale lithography of chalcoge-nides.19 However, the surface roughness measured at the topsurface of the lenses is undesirably high (∼50 nm).
3.5. Origin of Roughness. The drawback in using manychalcogenide patterning techniques for fabricating opticalelements is the undesirably high roughness of the lensesmaking them less useful for optical applications.7,33 Tounderstand the origin of roughness in lenses patterned at3600 s exposure, we characterized the surface of the as-deposited and annealed chalcogenide films. The roughness ofthe as-deposited and annealed films was measured by opticalprofilometer across more than one sample. The roughness ofthe as-deposited films was found to be ∼5 ± 1 nm, and afterannealing, the roughness decreased to ∼2 ± 1 nm. This level ofroughness indicates the relatively smooth nature of theannealed chalcogenide films before exposure. The reductionin roughness upon annealing is not significant enough to drawmajor conclusions. However, the change can possibly beattributed to the stabilization (i.e., polymerization of molecularunits into the matrix reducing the number of homopolarbonds)23 of the film and filling of voids created during thedeposition process. Further, the AFM profiles of samples that
Figure 3. Remaining height as a function of developing time forexposed and unexposed regions of a sample exposed for 900 s inethanolamine.
Figure 4. Height difference between exposed and unexposed regionsafter 3 min of developing in ethanol amine plotted as a function ofexposure time. Height difference was measured using an AFM.
Figure 5. (a) Brightfield microscope image of fabricated array ofcylindrical microlens arrays in As2Se3 (inset shows grayscale softwaremask used). (b) Profilogram demonstrating the change of height in thefabricated structures in As2Se3 with gradual variation of the grayscalemask. It may be noted that in (b) the x axis (nm) and y axis(micrometer) scales are vastly different resulting in compression offeature widths.
ACS Applied Materials & Interfaces Research Article
dx.doi.org/10.1021/am401368e | ACS Appl. Mater. Interfaces XXXX, XXX, XXX−XXXD
had both exposed and unexposed regions used in Section 3.4were analyzed. The roughness in the unexposed and exposedregions of the films was measured at each exposure time andplotted (Figure 6). As is clear from the graph, the roughness
increases as a function of exposure time for exposed regions,while the roughness of unexposed regions stays more or lessconstant. From this one can conclude that the nanoscaleroughness originates from the exposure step of lithographicpatterning. However, certain bigger defects (>1 μm indiameter) are also observed. These defects can be attributedto the oxide phase As2O3 that arises on exposure of As2Se3 inthe presence of oxygen34 and can be potentially addressed byexposure in inert conditions.The roughness variation with exposure time can be explained
if we consider the chemical changes that occur upon exposureof the As2Se3 films to UV radiation. We have previouslyreported the chemical changes that occur in As2Se3 films onexposure to UV radiation using Raman spectra measurements.The homopolar bonds in the chalcogenides, namely, As−Asand Se−Se, decrease with increasing the UV exposure time.However, the heteropolar bonds between As and Se increase.The selective etching of the unexposed areas arises fromrelatively higher rate of dissolution of the homopolar bonds inthe developer.14 The origin of roughness after chemical etchingcould be due to a difference in etching rates of As−As bondsand Se−Se bonds. A similar observation was found for As2S3
films that were plasma-etched by Choi and co-workers.35 Theyhave attributed the surface roughness in As2S3 films to thedifferential chemical attack of As- and S-rich phases in thethermally deposited films. Although their observations are inthe case of plasma etching and for the As−S system, one canmake a parallel argument considering the origin of roughness inthe exposure step. In our case, As2Se3 film regions exposed toradiation contain AsSe3 pyramids, As4Se3 units, and Se8 rings.Each of these contain As−As bonds and Se−Se bonds indifferent proportions, thus creating As-rich phases and Se-richphases. The differential etching of the As−As and Se−Se bondsimplies a differential etching of the above phases, and thenanoscale distribution of the As-rich and Se-rich phases causesa corresponding nanoscale roughness.Other researchers have also observed the change in
roughness in chalcogenide photoresists due to etching.36,37
Increase in the roughness in developed regions is due to thespatial variations in etching rate arising from nanostructuriza-tion in chalcogenides. However Dan’ko et al. have consideredthe case of photoinduced positive etching, i.e., the increasedetching rate in areas that are exposed to light during etching.Koreshev and Ratushnyi37 have also found an increase inroughness in unexposed developed films related to thenanostructural variations caused by initial cluster structure ofthe chalcogenide films. Their results related to exposeddeveloped films is relevant to the minimization of roughnessin lens arrays and will be discussed in the next section.
3.6. Minimization of Roughness in Lens Arrays. Asdiscussed previously, rough surfaces cause adverse consequen-ces for the focusing effect of the chalcogenides lenses and arethus undesirable for optical applications. Thus, a goodpatterning technique for chalcogenide lens arrays should resultin relatively smooth and curved surfaces. Figure 7A and B showoptical profilometer scans of the lens arrays exposed for 900and 1800 s, respectively. The profile of these lenses was fittedto a smooth function to calculate the roughness in a lenspattern. The roughness of lenses patterned at 900 and 1800 sexposure time was 1.0 ± 0.5 nm and 14 ± 1 nm, respectively.The 3D profile of the 900 s exposed lens array clearly illustratesthat the lenses are smoother with less defects compared to thelenses patterned at the 1800 s exposure time. It is to be notedthat the roughness or deviation from smooth structures in thecase of the 900 s exposure is different from the roughnessmeasured for blank exposed films. This may be due to the lowerexposure intensity at grayscale values lower than white in thelens structures resulting in a lower local exposure dose.However, if only this effect is considered, the roughness of the1800 s exposed lens arrays would have also decreased. This not
Figure 6. Plot of roughness after developing as a function of exposuretime.
Figure 7. Optical profilometer image of lens with (A) 900 s exposure time and (B) 1800 s exposure time. Inset in panel (A) shows the grayscaledigital mask used.
ACS Applied Materials & Interfaces Research Article
dx.doi.org/10.1021/am401368e | ACS Appl. Mater. Interfaces XXXX, XXX, XXX−XXXE
being the case, it is possible that the surface distribution ofnanophases does not increase linearly in this range of exposuredose.In this context, the work by Koreshev and Ratushnyi37
reveals that the roughness of films exposed to form relief phaseholograms using energies up to 200 mJ/cm2 lies between theroughness of unexposed developed films and unexposedundeveloped films. This is because of a decrease in thenanostructurization. This is contrary to our observed trend ofroughness in films at blank (white) exposure times between 900and 3600 s, i.e., exposure dose between 3150 and 12600 mJ/cm2. However, it can serve to explain the observed difference inroughness between grayscale-patterned lens arrays and blankexposure films. At grayscale values below 255, the lowerexposure dose might lead to a phase distribution of a muchlower length scale than at higher exposure doses, thus resultingin a lower roughness than expected from the roughness trend athigher exposure doses. A further understanding of the chemicalchanges that occur on exposure to UV light at differentexposure doses is required in order to optimize both roughnessand lens height.3.7. Patterning of Lens Arrays: Fabrication of Convex
and Concave Lenses. Having optimized the grayscalelithography parameters (developer, ethanolamine; developingtime, 3 min; exposure time, 900s), we attempted the fabricationof chalcogenide lens arrays. From an application point of view,both concave and convex structures are important. Concavestructures can act as waveguides, and convex lenses can focuslight in the IR region. By using a negative of the mask(substituting grayscale value x by 255 − x), we were able tofabricate both structures as shown in Figure 8. The 3D profilesobtained from optical profilometer are shown on the right and
illustrate a relatively smooth profile for both concave andconvex lenses.
3.8. Focal Length of Lenses. The dimensions and profileof the convex lens array were used to calculate the effectivefocal length. The focal length of the spherical lenses can becalculated using the following equation38
h n2 ( 1)
where h represents the microlens thickness, d represents thediameter of the microlens, n represents the refractive index ofthe As2Se3 at 3 μm, which is 2.78. The dimension of the plano−convex lens was obtained from the optical profilometry graphshown in Figure 9. A plano−convex lens array with a very longfocal length of ∼9.3 mm with a surface roughness less than 5nm could thus be fabricated using grayscale masklesslithography.
4. CONCLUSIONSMaskless grayscale lithography and wet etching using ethanol-amine have been successfully used for the fabrication of smooth3D optical structures in amorphous As2Se3 films for IR opticsapplications. This is a direct and simple single lithographic stepfabrication process that allows variation of thickness across amicrolens array in a controllable reproducible manner. Theexposure and etching parameters were optimized to result insmooth reproducible and periodic lens structures. Cylindricallenses and concave and convex periodic arrays were fabricatedwith minimal roughness on an ∼1 cm2 area. The focal length ofthe plano−convex lens was calculated to be ∼9.3 mm,establishing the utility of these lens arrays for optical focusing
Figure 8. Optical profilometer image of (A) convex microlens arrays and their (B) 3D view. (C) Concave microlens arrays and their (D) 3D view(insets in panels (A) and (C) show the grayscale mask used).
ACS Applied Materials & Interfaces Research Article
dx.doi.org/10.1021/am401368e | ACS Appl. Mater. Interfaces XXXX, XXX, XXX−XXXF
applications in the IR region. It is to be noted that while wehave demonstrated lens arrays having a single repeating pattern,it is possible to vary the dimensions and thickness, as well as thetype of pattern across the array, by using the same method. Thedifference between roughness on a blank exposed As2Se3 filmand the roughness of the lens patterned at the same exposuretime of 900 s is an interesting observation that can potentiallylead to better optimization of the exposure dose for smooth andtall structures.
■ AUTHOR INFORMATIONCorresponding Author*E-mail: [email protected] ContributionsThe manuscript was written by contributions of all authors. Allauthors have given approval for the final version of themanuscript.NotesThe authors declare no competing financial interest.
■ ACKNOWLEDGMENTSWe acknowledge the support of the Department of Science andTechnology (DST) to the Unit on Soft Nanofabrication at IITKanpur and Defense Research and Development Organization,New Delhi, India. We are thankful to Satinder Kumar Sharma,IIT Mandi for discussions.
■ REFERENCES(1) Zakery, A.; Elliott, S. R. J. Non-Cryst. Solids 2003, 330, 1−12.(2) Shimakawa, K.; Kolobov, A.; Elliott, S. R. Adv. Phys. 1995, 44,475−588.(3) DeCorby, R. G.; Ponnampalam, N.; Pai, M. M.; Nguyen, H. T.;Dwivedi, P. K.; Clement, T. J.; Haugen, C. J.; McMullin, J. N.; Kasap,S. O. IEEE J. Sel. Top. Quantum Electron. 2005, 11, 539−546.(4) Klebanov, M.; Lyubin, V.; Kirzhner, M. G.; Abdulhalim, I. J. Appl.Phys. 2013, 113, 033503−6.(5) Abdulhalim, I.; Gelbaor, M.; Klebanov, M.; Lyubin, V. Opt. Mater.Express 2011, 1, 1192−1201.(6) Kaganovskii, Y.; Beke, D. L.; Kokenyesi, S. Appl. Phys. Lett. 2010,97, 061906−3.(7) Kovalskiy, A.; Vlcek, M.; Jain, H.; Fiserova, A.; Waits, C. M.;Dubey, M. J. Non-Cryst. Solids 2006, 352, 589−594.(8) Tsiulyanu, D. Non-Crystalline Materials for Optoelectronics;Optoelectronic Materials and Devices Series; INOE PublishingHouse: Bucharest, Romania, 2004; Vol. 1, p 297.(9) Vlcek, M.; Jain, H. J. Optoelectron. Adv. Mater 2006, 8, 2108−2111.(10) Bryce, R. M.; Nguyen, H. T.; Nakeeran, P.; DeCorby, R. G.;Dwivedi, P. K.; Haugen, C. J.; McMullin, J. N.; Kasap, S. O. J. Vac. Sci.Technol., A 2004, 22, 1044−1047.
(11) Bureau, B.; Zhang, X. H.; Smektala, F.; Adam, J.-L.; Troles, J.;Ma, H.-l.; Boussard-Pledel, C.; Lucas, J.; Lucas, P.; Le Coq, D.; Riley,M. R.; Simmons, J. H. J. Non-Cryst. Solids 2004, 345−346, 276−283.(12) van Popta, A.; DeCorby, R.; Haugen, C.; Robinson, T.;McMullin, J.; Tonchev, D.; Kasap, S. Opt. Express 2002, 10, 639−644.(13) Shankar, M.; Willett, R.; Pitsianis, N.; Schulz, T.; Gibbons, R.;Te Kolste, R.; Carriere, J.; Chen, C.; Prather, D.; Brady, D. Appl. Opt.2008, 47, B1−B10.(14) Kovalskiy, A.; Cech, J.; Vlcek, M.; Waits, C. M.; Dubey, M.;Heffner, W. R.; Jain, H. J. Micro/Nanolithogr., MEMS, MOEMS 2009,8, 043012−043012.(15) Eisenberg, N.; Manevich, M.; Arsh, A.; Klebanov, M.; Lyubin, V.J. Optoelectron. Adv. Mater 2002, 4, 405−407.(16) Eisenberg, N.; Klebanov, M.; Lyubin, V.; Manevich, M.; Noach,S. J. Optoelectron. Adv. Mater. 2000, 2, 147−152.(17) Manevich, M.; Klebanov, M.; Lyubin, V.; Varshal, J.; Broder, J.;Eisenberg, N. Chalcogenide Lett. 2008, 5, 58−60.(18) Manevich, M.; Klebanov, M.; Lyubin, V.; Varshal, J.; Border, J.;Eisenberg, N. Chalcogenide Lett. 2008, 5, 61−64.(19) Eisenberg, N.; Manevich, M.; Arsha, A.; Klebanova, M.;Lyubina, V. Chalcogenide Lett. 2005, 2, 35−37.(20) Orava, J.; Kohoutek, T.; Greer, A. L.; Fudouzi, H. Opt. Mater.Express 2011, 1, 796−802.(21) Bulanovs, A.; Gerbreders, V.; Kirilovs, G.; Teteris, J. Cent. Eur. J.Phys. 2011, 9, 1327−1333.(22) Dan’ko, V. A.; Indutnyi, I. Z.; Min’ko, V. I.; Shepelyavyi, P. E.Optoelectron., Instrum., Data Process. 2010, 46, 483−490.(23) Dan’ko, V. A.; Indutnyi, I. Z.; Min’ko, V. I.; Shepelyavyi, P. E.;Bereznyova, O. V.; Lytvyn, O. S. Semiconductors 2012, 46, 504−508.(24) Rammohan, A.; Dwivedi, P. K.; Martinez-Duarte, R.; Katepalli,H.; Madou, M. J.; Sharma, A. Sens. Actuators, B 2011, 153, 125−134.(25) Nemec, P.; Frumar, M.; Jedelsky, J.; Jelínek, M.; Lancok, J.;Gregora, I. J. Non-Cryst. Solids 2002, 299, 1013−1017.(26) Dwivedi, P. K.; Sharma, S. K.; Rammohan, A.; Sharma, A. AIPConf. Proc. 2011, 1349, 555−556.(27) Antoine, K.; Jain, H.; Vlcek, M. J. Non-Cryst. Solids 2006, 352,595−600.(28) Tanaka, K.; Saitoh, A.; Terakado, N. J. Optoelectron. Adv. Mater.2006, 8, 2058−2065.(29) Ramachandran, S.; Pepper, J. C.; Brady, D. J.; Bishop, S. G. J.Lightwave Technol. 1997, 15, 1371−1377.(30) Carlie, N. A. A Solution-Based Approach to the Fabrication ofNovel Chalcogenide Glass Materials and Structures. Ph.D. Thesis,Clemson University, March 2010.(31) Mamedov, S.; Mikhailov, M. J. Non-Cryst. Solids 1997, 221,181−186.(32) Michailov, M. D.; Mamedov, S. B.; Tsventarnyi, S. V. J. Non-Cryst. Solids 1994, 176, 258−262.(33) Eggleton, B. J.; Luther-Davies, B.; Richardson, K. Nat. Photonics2011, 5, 141−148.(34) Sanchez, E. A.; Waldmann, M.; Arnold, C. B. Appl. Opt. 2011,50, 1974−1978.(35) Choi, D.-Y.; Madden, S.; Rode, A.; Wang, R.; Bulla, D.; Luther-Davies, B. J. Non-Cryst. Solids 2008, 354, 5253−5254.(36) Dan’ko, V.; Indutny, I.; Myn’ko, V.; Shepeliavyi, P.; Lykanyuk,M.; Lytvyn, O. J. Non-Oxide Glasses 2012, 3, 13−18.(37) Koreshev, S. N.; Ratushnyĭ, V. P. Opt. Spectrosc. 2009, 106,288−292.(38) Savastru, D.; Miclos, S.; Savastru, R. J. Optoelectron. Adv. Mater.2005, 7, 1909−1913.
Figure 9. Profile of plano−convex lens having a 150 μm diameter anda 170 nm height as measured by optical profilometry.
ACS Applied Materials & Interfaces Research Article
dx.doi.org/10.1021/am401368e | ACS Appl. Mater. Interfaces XXXX, XXX, XXX−XXXG